Review Antireﬂective Coatings: Conventional Stacking Layers and Ultrathin Plasmonic Metasurfaces, A Mini-Review
Mehdi Keshavarz Hedayati 1,* and Mady Elbahri 1,2,3,* 1 Nanochemistry and Nanoengineering, Institute for Materials Science, Faculty of Engineering, Christian-Albrechts-Universität zu Kiel, Kiel 24143, Germany 2 Nanochemistry and Nanoengineering, Helmholtz-Zentrum Geesthacht, Geesthacht 21502, Germany 3 Nanochemistry and Nanoengineering, School of Chemical Technology, Aalto University, Kemistintie 1, Aalto 00076, Finland * Correspondence: firstname.lastname@example.org (M.K.H.); mady.elbahri@aalto.ﬁ (M.E.); Tel.: +49-431-880-6148 (M.K.H.); +49-431-880-6230 (M.E.)
Academic Editor: Lioz Etgar Received: 2 May 2016; Accepted: 15 June 2016; Published: 21 June 2016
Abstract: Reduction of unwanted light reﬂection from a surface of a substance is very essential for improvement of the performance of optical and photonic devices. Antireﬂective coatings (ARCs) made of single or stacking layers of dielectrics, nano/microstructures or a mixture of both are the conventional design geometry for suppression of reﬂection. Recent progress in theoretical nanophotonics and nanofabrication has enabled more ﬂexibility in design and fabrication of miniaturized coatings which has in turn advanced the ﬁeld of ARCs considerably. In particular, the emergence of plasmonic and metasurfaces allows for the realization of broadband and angular-insensitive ARC coatings at an order of magnitude thinner than the operational wavelengths. In this review, a short overview of the development of ARCs, with particular attention paid to the state-of-the-art plasmonic- and metasurface-based antireﬂective surfaces, is presented.
Keywords: antireflective coating; plasmonic metasurface; absorbing antireflective coating; antireflection
1. Introduction Refection of light (light-bending power) off the boundary (or at the interface) of two mediums is a desired phenomenon in mirrors but it is unfavorable in telescopes , lenses, and glasses  where it is considered as optical loss (absorption). For the latter cases, there has been an ongoing effort to reduce reﬂection by using some coating and patterns on the reﬂective surface, which is known as antireﬂective (or antireﬂection) coating (ARC). The development of ARCs began with Rayleigh in 1879, when he proposed that the reﬂectivity off the outer surface of an object could be reduced on the condition that the transition of refractive index (RI) between the object and surrounding medium is small . Following the proposal of Rayleigh, English lens designer H. Dennis Taylor in 1892 saw that tarnished camera lenses permit photography with less exposure . He discovered a decline in reﬂection linked to the coating (tarnish) on a glass surface . This observation turned into a method of ARC development when F. E. Wright intentionally tarnished glass via chemical approaches. He described the mechanism of the anti-glare properties of the coating in terms of gradual RI transition from glass to air due to tarnishing . Throughout the last century, various methods and strategies have been developed in order to lessen the reﬂection including (but not limited to) single-, double- or multiple layer ARCs as well as structuring/patterning of the surface. All of these methods are referred to throughout this review as conventional approaches as the principle and progress of each method is discussed.
Materials 2016, 9, 497; doi:10.3390/ma9060497 www.mdpi.com/journal/materials Materials 2016, 9, 497 2 of 22
The rapid development of modern optoelectronic devices such as displays, touchscreens and super-compact cameras, among others, place new demands on the ARC industry. The optic market requires three properties in particular of the ARCs: (1) ultrathin thickness; (2) insensitivity to the angle of incidence (non-iridescent); and (3) broadband. These requirements have recently been met by the emergence of the plasmonic and metasurface concept which is discussed in the present review.
2. Conventional Antireﬂective Coatings (ARCs)
2.1. Single-Layer ARC In principle, one can calculate the intensity of the light which reﬂects off any surface (interface of any medium with surrounding environment) with the Fresnel equation . Accordingly, a non-absorbing substance with refractive index (RI) equals ns at a desired wavelength; the RI and the thickness of the coating (also known as quarter-wavelength ARC) should fulﬁll the following conditions in order to reduce the reﬂection of the substrate down to zero at that wavelength: ? narc “ ns.nenv (1)
λ darc “ (2) 4 ˆ narc in which nenv and narc are the RI of the surrounding medium and ARC and darc is the thickness of the ARC, respectively. Note that the above equations are only valid for a homogeneous and non-absorbing medium; otherwise, the calculation gets more complicated due to the loss at each medium. For silicon (as the main absorbing material in the photovoltaic industry), in the middle of the visible spectrum 550 nm, one needs to deposit a 68 nm coating with an RI of 2.02 (e.g., Si3N4 ). Such a coating provides the reﬂection dip at 550 nm, whereas the average reﬂection through the visible spectrum would be 5.3%. The major problem of single-layer quarter-wavelength ARCs is that they reduce the reﬂectivity for limited (almost single) wavelengths and incidence angle (their performance vanishes at glazing incidence angle). The reason is that the optical path length of the incident light differs at a glazing incidence relative to the norm and the phase difference of reﬂected wave and incident wave will therefore not cancel each other out (i.e., no complete destructive interference). Moreover, a limited number of materials with low RI ﬁnd single-layer ARCs for many transparent media (generally low RI substrates) difﬁcult. For instance, for glass (n = 1.5), the RI of the coating (according to Equation (1)) should be 1.22. In nature, such a material does not exist and therefore any material with an RI close to this value would have to be used which certainly does not reduce the reﬂection efﬁciently. One solution to this problem is using composite single layer ARCs in which the RI of the coating can be tuned by varying the ratio (ﬁlling factor) of the components of the composite. This calculation can be made by effective medium approximation such as the Maxwell-Garnet equation  (which will not be discussed in detail here; readers are thus referred to  and the references therein.):
εe f f ´ εm ε ´ ε “ f i m (3) ε ` 2ε i ε ` 2ε ˜ e f f m ¸ ˆ i m ˙ in which εe f f , εi and εm are the dielectric constant of the effective medium (composite), inclusion and matrix, respectively whereas fi is the ﬁlling factor (volue fraction) of the inclusion. Note that the RI of a nonmagnetic medium has the following relationship with the dielectric constant: ? n “ ε (4)
Here, the RI of the composite is determined by the mixing of the RI of the components: the higher the volume fraction of the lower RI constituents, the lower the RI of the composite. Accordingly, Materials 2016, 9, 497 3 of 21
Here, the RI of the composite is determined by the mixing of the RI of the components: the higher Materials 2016, 9, 497 3 of 22 the volume fraction of the lower RI constituents, the lower the RI of the composite. Accordingly, Polman and co-workers developed a single-layer ARC which is made by sol–gel chemistry and large- areaPolman substrate-conformal and co-workers soft-imprint developed atechnology single-layer (Figure ARC 1a). which The isprinted made pattern by sol–gel is composed chemistry of and120 nmlarge-area tall silica substrate-conformal nano-cylinders with soft-imprint a diameter technology of 245 nm (Figurepossessing1a). Thean effective-index printed pattern (n is = composed1.20) ARC thatof 120 diminishes nm tall silica the nano-cylindersaverage double-sided with a diameterreflection ofof 245glass nm from possessing 7.35% to an 0.57% effective-index (Figure 1b). (n The= 1.20) RI ofARC the thatcoating diminishes indeed can the be average tuned to double-sided realize a broad reﬂection range of of values glass from(1.002 7.35% < n < 1.44, to 0.57% in theory) (Figure which1b). expandThe RI of the the application coating indeed of the can betechnique tuned to for realize other a broadreflective range materials, of values (1.002too . < n
Figure 1. (a) Schematic of the one-step nanoimprint lithography fabrication method. The spin-coated Figure 1. (a) Schematic of the one-step nanoimprint lithography fabrication method. The spin-coated sol−gel is patterned by a PDMS stamp to create an effective-index AR coating and SEM image of the sol´gel is patterned by a PDMS stamp to create an effective-index AR coating and SEM image of the sol−gel nanocylinder array on a Si substrate, showing the cylindrical shape of the nanoparticles and sol´gel nanocylinder array on a Si substrate, showing the cylindrical shape of the nanoparticles and the 30 nm residual sol−gel layer (cleaved sample imaged under 52°); (b) Measured total reflection the 30 nm residual sol´gel layer (cleaved sample imaged under 52˝); (b) Measured total reflection spectra for a flat reference (blue), one-side patterned (red), and two-side patterned (black) glass spectra for a flat reference (blue), one-side patterned (red), and two-side patterned (black) glass substrates. substrates. The dashed lines show the calculated reflection. (Adapted with permission from . The dashed lines show the calculated reflection. (Adapted with permission from . Copyright Copyright 2015, American Chemical Society); (c) Cross-section SEM image of nanoparticle 2015, American Chemical Society); (c) Cross-section SEM image of nanoparticle antireflective coating; antireflective coating; (d) Experimental reflection spectra of glass and ARC and theoretically (d) Experimental reflection spectra of glass and ARC and theoretically calculated reflection spectra for calculated reflection spectra for ARC and MgF2 . (Adapted with permission from . Copyright ARC and MgF2 . (Adapted with permission from . Copyright 2012, American Chemical Society). 2012, American Chemical Society). 2.2. Double-Layer ARC
Double-layer or V-shaped (because of the V-shape of their proﬁle [32–35]) ARCs are very common in the industry for reducing reﬂection of a coating from a speciﬁc wavelength. In the case of double-layer ARCs, the upper ﬁlm facing the air usually has the lowest refractive index, and the Materials 2016, 9, 497 4 of 21
2.2. Double-Layer ARC MaterialsDouble-layer2016, 9, 497 or V-shaped (because of the V-shape of their profile [32–35]) ARCs are 4very of 22 common in the industry for reducing reflection of a coating from a specific wavelength. In the case of double-layer ARCs, the upper film facing the air usually has the lowest refractive index, and the other layer(s) is (are) made successively based on the ascending order of their refractive indices. other layer(s) is (are) made successively based on the ascending order of their refractive indices. In In double-layer ARCs, the interference conditions should be fulﬁlled in order to destructively cancel double-layer ARCs, the interference conditions should be fulfilled in order to destructively cancel the the bouncing back waves off the surface of the substance. Therefore, the thickness of each single layer bouncing back waves off the surface of the substance. Therefore, the thickness of each single layer is is usually quarter or half of the operational wavelength ( λ and λ ). If the optical thickness of the layers usually quarter or half of the operational wavelength (4 2 ). If the optical thickness of the in double-layer geometry obeys the following equations: 4 2 layers in double-layer geometry obeys the following equations:
n1 ˆ d1 “ n2 ˆ d2 (5) × = × (3) thethe necessarynecessary andand sufﬁcientsufficient indexindex conditioncondition inin orderorder toto reducereduce reﬂectionreflection down down to to zero zero is is [ 33:]: